MJCCA9 – 694 ISSN 1857-5552 e-ISSN 1857-5625
Received: April 4, 2014 UDC: 547.979.8:544.723.3
Accepted: November 10, 2014 Original scientific paper
DESORPTION OF β-CAROTENE FROM BENTONITE ADSORBENT
UNDER MICROWAVE IRRADIATION
Tatjana Novaković1, Ljiljana Rožić1*, Srdjan Petrović1
, Dragomir Stanisavljev2
University of Belgrade, Institute of Chemistry, Technology and Metallurgy, Department of Catalysis and Chemical Engineering, Njegoševa 12, Belgrade, Republic of Serbia
University of Belgrade,Faculty of Physical Chemistry, Studentski trg 12-16, Belgrade, Republic of Serbia
The desorption behavior of β-carotene from a bentonite adsorbent under microwave irradiation in isopropanol was studied as a function of temperature and different initial loading concentrations. A first-order, two-component, three-parameter model described the desorption kinetics with a coefficient of de-termination R2 > 0.9932, and the β-carotene desorption process under microwave irradiation was con-trolled by both rapid and slow desorption. The activation energies of β-carotene desorption for the rapid and slow desorption processes were 19.61 and 53.04 kJ mol–1, respectively. It was observed that the de-sorption equilibrium data fitted well to both the Freundlich and Langmuir isotherms. The data obtained from the desorption-isotherm model were used to determine the thermodynamic parameters. The positive value of free energy indicates the non-spontaneity of β-carotene desorption. The change in entropy rela-tive to the enthalpy of desorption reveals that the reaction is physical in nature.
Keywords:β-carotene; desorption; bentonite; microwave irradiation; kinetics
ДЕСОРПЦИЈА НА β-КАРОТЕН ОД БЕНТОНИТСКИ АТСОРБЕНТ ВО УСЛОВИ НА МИКРОБРАНОВА ИРАДИЈАЦИЈА
Десорпциското однесување на β-каротенот од бентонитски атсорбент беше истражувано во услови на микробранова ирадијација како функција на температурата и различни концентрации на полнењето. Кинтетички двокомпонентен модел од прв ред со три параметри ја опишува десорпциската кинетика со коефицинет на корелација R2 > 0.9932. Десорпцискиот процес на β -каротенот во услови на микробранова ирадијација е контролиран и со брза и со бавна десорпција. Активациските енергии на десорпцијата на β-каротенот за брзата и за бавната десорпција соодветно изнесуваат 19,61 kJ mol–1 и 53,04 kJ mol–1. Забележано е дека десорпциската рамнотежа добро се вклопува во изотермите на Freundlich и на Langmuir. Добиените податоци на моделот на десорпциската изотерма се употребени за определување на термодинамички параметри. Позитивната вредност на слободната енергија укажува на неспонтаност на десорпцијата на β -каротенот. Промената на ентропијата во однос на енталпијата укажува дека десопцијата по природа е физичка.
Клучни зборови:β-каротен; десорпција; бентонит; микробранова ирадијација; кинетика
β-Carotene is an important member of the carotenoid family of orange-colored pigments,
the process. A number of adsorption/desorption processes involving the removal of colored pig-ments have been observed to exhibit biphasic be-havior, with a rapidly desorbing phase followed by a fraction that desorbs more slowly. Most previous studies have focused on the removal of β-carotene and chlorophyll from various types of oils by acid-activated bentonite [3–9]. These studies reported that the rate of adsorption is controlled by mass transfer because the adsorption rate of β-carotene is very fast compared to the rate of its transfer from the bulk oil to the clay surface.
The first (fast) step of adsorption represents the chemical interaction between the acid centers on the bentonite surface and β-carotene, whereas the second (slow) step may indicate the physical adsorption of β-carotene onto the molecules that are adsorbed in the first step. The heterogeneity of the active centers explains the gradual increase in adsorption of β-carotene with increasing tempera-tures at different clay/oil ratios, because a propor-tion of these centers are activated at higher temper-atures [3, 6]. The dependence of the adsorp-tion/desorption rates on temperature is determined by the activation energy, which essentially de-scribes how the chemical rate constants vary with temperature.
As edible oils contain a mixture of organic compounds (carotenoids, such as β-carotene and their derivatives, chlorophyll, tocopherols, and gossypol), fundamental studies on isolated mole-cules are scarce, and researchers tend to focus on the efficiency of the adsorption/desorption of com-pounds and the decrease in time and energy con-sumption [7, 9, 10].
Only a few attempts have been made to de-scribe the adsorption of β-carotene on acid-activated bentonite at low temperatures, using ace-tone, xylene, n-hexane, or isopropanol as solvents [6, 7, 11, 12]. Muhammad et al. have shown that the adsorption of β-carotene using isopropanol is higher than using n-hexane as a solvent because of the low polarity index of n-hexane compared to isopropanol. Therefore, the stronger bond between
β-carotene and n-hexane inhibits the transfer of carotene to the adsorbent .
Microwave heating is a widely accepted, nonconventional energy source for inorganic syn-thesis  and different physicochemical process-es such as regeneration , extraction [15, 16], adsorption , and desorption . The efficien-cy of microwave-based processes is not only re-flected in the reduction in reaction time, it is also known to significantly accelerate the rate of chem-ical reactions and physicochemchem-ical processes,
re-sult in higher yields and improve the properties of the products .
Although extensive studies on the effects of microwave heating various physicochemical pro-cesses have been reported, the influence of micro-wave heating on the desorption processes of β -carotene from bentonite adsorbents has not yet been investigated.
In this study, the effect of different experi-mental parameters, that is, the desorption tempera-ture and various initial concentrations of β -carotene, on the fast- and slow-desorption process-es induced by microwave heating were studied by performing simulations based on a kinetic model. A first-order, two-component, three-parameter model was applied to fit the experimental data. The kinetics and thermodynamic parameters, such as the Gibbs free energy, enthalpy, and entropy, were also calculated. These approaches provide greater insight into the characteristics of β-carotene de-sorption from acid-activated bentonite. The results help to understand the reaction mechanism of β -carotene during microwave heating and promote the application of β-carotene in the food industry.
The results of our previous investigations on the modelling and optimization of bentonite activa-tion through a response surface methodology  were applied to modify bentonite, which was used as the starting material in the current study. Acid-activated bentonite (AABent) obtained under these optimal conditions, with a particle size less than 75 m (–200 mesh ASTM), has an average chemical composition (% by wt.) of SiO2 73.66, Al2O3 12.28,
Fe2O3 4.73, CaO 0.70, MgO 1.99, Na2O 0.60, K2O
0.30, and TiO2 0.57, as well as an ignition upon loss
of 5.17. Mineralogical analysis confirmed that AABent consisted predominantly of smectite and contained a substantial amount of quartz impurities as well as minor amounts of feldspar. Anhydrous o -xylene, isopropanol, and β-carotene were purchased from Sigma–Aldrich (USA).
2.2. Nitrogen adsorption
The specific surface area, pore diameter, and total pore volume of the prepared AABent were measured by N2 adsorption–desorption isotherms
cal-culated by fitting the adsorption data to the linear range of the BET equation [relative to p/p0 (0.05– 0.35)]. The pore size distribution was calculated according to the BJH method using N2 desorption
2.3. Adsorption of β-carotene onto acid activated bentonite
In a 250 ml conical flask, AABent (10 g) was initially saturated with different concentrations (389, 581, and 658 mg l–1) of β-carotene solution in
o-xylene. The saturation reaction was conducted in a temperature-controlled water-bath shaker at 338 K and 150 rpm for 90 min in order to reach equi-librium . To establish thermal equiequi-librium be-fore adsorption, the flask containing the solution was agitated for 15 min in a water bath at the de-sired temperature, and the AABent was then added to the solution. After a predetermined amount of time, the samples were filtered immediately and the supernatant solution was analyzed using a UV/Vis spectrophotometer (Thermo Electron Cor-poration, Evolution 500). The absorbance of the β -carotene was measured before and after adsorption at a wavelength of 457 nm. The absorbance values of β-carotene could be transformed to β-carotene concentrations using the calibration curve.
The obtained result, reported as the amount of β-carotene adsorbed per gram of AABent, was used as the initial concentration in the desorption experiments.
2.4. Desorption of β-carotene under microwave irradiation
Desorption of β-carotene from AABent satu-rated with different β-carotene concentrations (3.89, 5.81, and 6.58 mg β-carotene per gram ben-tonite; denoted as samples 1, 2, and 3, respective-ly) was carried out using a CEM-focused micro-wave reactor (Discovery, Corp. Matthews, North Carolina, US) with an adjustable power and
con-tinuous microwave power output operated at 2.45 GHz. All experiments were performed in a cylin-drical glass cell with diameter d = 9 mm and height
H = 45 mm. To maintain constant microwave irra-diation and a constant temperature during the pro-cess, the temperature of the cell was externally controlled. The temperature of the solution was measured with a commercial fiber optic sensor. To measure the desorption kinetics, isopropanol solu-tion (10 ml) was added to a cylindrical glass cell and then heated in the microwave reactor at a con-stant microwave power of 80 W. After reaching the required experimental temperature, AABent (0.4 g) with different β-carotene concentrations was placed in the cell. The samples were with-drawn at specified time intervals and analyzed us-ing a UV/Vis spectrophotometer at λmax = 457 nm. The amount of β-carotene remaining on the adsor-bent, qt (mg g–1), was calculated using the mass-balance equation:
m C C V q
where qi is the initial solid-phase β-carotene concen-tration (mg g–1), Ct is the β-carotene concentration in solution (mg l–1) at any time, Ci is the initial β -carotene concentration in solution (mg l–1), V is the volume of the solution, and m is the adsorbent mass.
3. RESULTS AND DISCUSSION
3.1. Textural properties of bentonite adsorbents
The textural properties of the as-prepared AABent and AABent with various initial β -carotene loading concentrations are presented in Table 1. Adsorption analysis revealed that all of the samples yielded type IV isotherms , which are indicative of mesoporous materials (Figure 1).
T a b l e 1
Textural properties of bentonite adsorbents as a function of the initial loading concentration of β-carotene
Sample BET surface area (m2 g–1)
Pore volume (cm3g–1)
Micropore volume (cm3 g–1)
Pore diameter (nm)
AABent 202 0.246 0.0913 3.71
Sample 1 175 0.231 0.0659 3.62
Sample 2 166 0.225 0.0634 3.64
The general shape of the isotherms did not change after β-carotene adsorption; however, a slight decrease in the amount of adsorbed nitrogen was observed. All of the isotherms were reversible at a low equilibrium pressure. However, under high pressure, an H3 hysteresis loop was observed , indicating that the pores were shaped as slits or ink bottles (pores with narrow necks and wide bodies).
Sample 3 Sample 2 Sample 1
0.0 0.2 0.4 0.6 0.8 1.0
Fig. 1. Adsorption–desorption isotherms of samples 1, 2, and 3 as well as AABent
Comparison of the results (Table 1) shows that the specific surface area and the total pore volume decreased as the initial loading concentra-tion of β-carotene increased. The micropore vol-umes of AABent and samples 1, 2, and 3 exhibited a behavior that was very similar to that of the total pore volume. However, the mean pore diameter remained constant, indicating that the preparation procedure did not alter the primary structure of the support. Thus, only partial filling of pores was ob-served, owing to the adsorption of β-carotene. Changes in the surface area, micropore volume, and pore volume indicate that the adsorption may have occurred on the external surface, as there is no change in pore diameter.
3.2. Desorption profile
The extent of β-carotene desorption from samples 1, 2, and 3 under microwave irradiation was studied as a function of time under different conditions, that is, with different initial β-carotene concentrations and desorption temperatures. The β -carotene desorption profiles were similar for all of the systems (Fig. 2 and Fig. 3).
Fig. 2. Desorption profile of β-carotene as a function of the contact time at various desorption temperatures
Fig. 3. Desorption profile of β-carotene as a function of the contact time at various initial loading concentrations
recovery, indicating that desorption of β-carotene from samples 1, 2, and 3 under microwave irradia-tion was also an endothermic process.
The desorption profiles of β-carotene from AABent at various initial concentrations (Fig. 3) reveal that increasing the concentration of β -carotene leads to a decrease in the β-carotene de-sorption rate.
3.3. Desorption kinetics
A first-order, two-component, three-para-meter model was used to predict the β-carotene desorption kinetics. The model developed by John-son and Weber  is defined as follows:
q s r
were Φs is the slowly desorbing fraction, (1–Φs) is the rapidly desorbing fraction, and ks and kr (min–1) are the rate constants of slow and rapid desorption, respectively. This model was fitted to desorption kinetics data using the non-linear regression meth-od. The values of ks, kr, and ΦSwere obtained by minimizing the sum of the squares of the differ-ences between the experimental and calculated values of qt/qi. The parameters obtained from the model are useful for distinguishing between the rapidly and slowly desorbing fractions. This model does not necessarily have a physical meaning, that is, it is uncertain whether the rapid and slow de-sorption processes correspond to physicochemical processes. The desorption parameters obtained from the model are shown in Table 2.
T a b l e 2
Desorption rate parameters for β-carotene as a function of temperature at an initial loading of 6.58 mg g–1 and as a function of the initial loading at 303 K
S kr (min–1) ks (min–1) R2 SSE Temperature (K)
298 0.9558 1.7170 0.00074 0.9959 2.8 10-5
303 0.9535 1.8197 0.00112 0.9965 5.1 10-6
308 0.9536 2.3029 0.00155 0.9981 2.9 10-6
313 0.9475 2.6955 0.00280 0.9932 1.1 10-5
Initial loading conc. (mg g–1)
3.89 0.9435 2.5495 0.00110 0.9999 1.9 10-7
5.81 0.9483 1.1248 0.00096 0.9989 1.9 10-6
6.58 0.9536 1.2160 0.00094 0.9969 4.5 10-6
It was observed that the model fitted the ex-perimental data well, with a high coefficient of determination, R2, greater than 0.9932. Also, the residual sum of squares (SSE) is a measurement of the discrepancy between the data and the estima-tion model. The very small SSE value shows that the experimental value was reasonably close to the predicted value.
Both the rapid and slow desorption rates and the slow desorption fraction were strong functions of desorption temperature and the initial loading concentration. The results show that, when the temperature increased from 298 to 313 K, the ks
and kr values increased from 0.000739 to 0.00280
min–1 and from 1.717 to 2.695 min–1, respectively. On the other hand, when the initial β-carotene loading concentration was increased, the desorp-tion was slow and the ks and kr values decreased
from 0.0011 to 0.00094 min–1 and from 2.549 to 1.216 min–1, respectively. An increase in the
de-sorption temperature resulted in a decrease in the values of Φs, whereas increasing the initial con-centration of β-carotene at 303 K is proportional to the change in Φs.
3.4. Arrhenius plot
The temperature dependence of the desorp-tion rates of the rapidly and slowly desorbing β -carotene fractions can be described by an Arrheni-us relationship [9, 23]:
RT E k
ks 0exp des , (3)
where k0 is the Arrhenius pre-exponential factor,
The equation can be rearranged as follows:
log kr or
RT E k
303 . 2 log
s . (4)
The activation energies of β-carotene de-sorption for both the rapid and slow processes were calculated from the slope of the plot of log kr or
log ks versus 1/T (Fig. 4).
Fig. 4. Arrhenius relationships between temperature and the rate constants of the rapid and slow desorption processes of β -carotene from AABent with different loading concentrations
The values of Edes obtained for the rapid and slow desorption processes were 19.61 and 53.04 kJ mol–1, respectively. These activation energy values are mainly for physical desorption mechanisms, and the whole desorption process could be finally controlled by diffusion. A higher activation energy was observed for the slow rate constant, confirm-ing that diffusion may have occurred through the mesopores with smaller pore diameters. The acti-vation energies obtained are higher than those cal-culated by Muhammad et al.  (Edes,rapid = 7.88 kJ mol–1 and Edes,slow = 44.47 kJ mol–1) for β-carotene desorption from a mesoporous carbon-coated monolith in the temperature range 303–323 K. However, the observed difference can be explained by the different experimental conditions used (mi-crowave irradiation) and the properties of the ad-sorbent.
3.5. Desorption isotherms
The desorption equilibrium data were fitted to the Freundlich and Langmuir models. The well-known logarithmic form of the Freundlich iso-therm is expressed as follows:
q log 1 log
log F , (5)
where qe is equilibrium solid-phase β-carotene concentration,Ce is equilibrium β-carotene concen-tration in solution, KF and n are Freundlich con-stants, with n indicating how favorable the adsorp-tion process will be and KF (mg [g (L mg–1)1/n]–1) representing the adsorption capacity of the adsor-bent. KF can be defined as the adsorption or
distri-bution coefficient and represents the quantity of β -carotene adsorbed onto AABent for a unit equilib-rium concentration. The slope of 1/n, which ranges between 0 and 1, is a measure of the adsorption intensity or surface heterogeneity, where values close to 0 indicate high heterogeneity . A value of 1/n below 1 indicates a normal Langmuir iso-therm, whereas 1/n values above 1 are indicative of cooperative adsorption. The plot of log qe versus log Ce yields a straight line with a slope of 1/n and an intercept of log KF.
The Langmuir model assumes that the sur-face of an adsorbent is homogeneous and that the adsorption energy is uniform for each adsorption site and solute uptake occurs by monolayer adsorp-tion. A linearized form of the Langmuir isotherm is expressed as follows:
e 1 1
C b b K q
where KL is the Langmuir equilibrium constant (L mg–1) and b is the monolayer capacity of the adsor-bent (mg g–1). The constants can be calculated from the slope and intercept of the straight line formed by plotting Ce/qe versus Ce. The essential
characteris-tics of the Langmuir isotherm can be expressed by a dimensionless constant called the separation factor, or equilibrium parameter, RL, defined by Weber and Chakkravorti  as follows:
0 L L
where C0 is the highest β-carotene concentration (mg l–1). The value of RL indicates the type of iso-therm that describes the desorption process: favor-able (0< RL<1), unfavorable (RL>1), linear (RL=1), or irreversible (RL=0) .
T a b l e 3
Freundlich and Langmuir isotherm parameters for desorption of β-carotene from bentonite adsorbents under microwave irradiation
Desorption system Langmuir model Freundlich model
(L mg–1) R
(mg [g(L/mg)1/n]–1) 1/n R
303 26.00 0.021 0.989 0.76 0.675 0.813 0.999 308 16.76 0.038 0.995 0.65 0.742 0.800 0.993 313 10.80 0.077 0.974 0.44 1.309 0.546 0.992
The Freundlich and Langmuir models yielded high R2 values, which were greater than 0.97 at all three temperatures studied, demonstrating that the desorption of β-carotene from a bentonite adsorbent can be described by these two models. For all of the desorption systems, the experimental data were ob-served to fit the Freundlich model better than the Langmuir model, as indicated by the higher R2 val-ues of the former. The relatively high non-linearity of the desorption isotherm may be attributed to the heterogeneity of the adsorption sites on the AABent surface , which suggests that some heterogeneity on the surface, or pores of the bentonite adsorbent, played a role in β-carotene desorption.
3.6. Desorption thermodynamics
The thermodynamic parameters that must be considered to evaluate desorption processes, such as changes in enthalpy (ΔH), entropy (ΔS), and Gibbs free energy (ΔG), were determined using data obtained from the Langmuir isotherm. The values of ΔH and ΔS can be computed using the following equation:
RT H R
ln , (8)
where R (8.314 J mol–1K–1) is the universal gas constant, T (K) is the absolute desorption tempera-ture, and KL (L mg–1) is the Langmuir isotherm constant. The values of ΔH and ΔS can be calculat-ed from the slope and intercept, respectively, of the van’t Hoff plot of ln KL versus 1/T (Fig. 5).
Fig. 5. Plot of ln KL versus 1/T used to estimate the
thermo-dynamic parameters of β-carotene desorption from AABent with different loading concentrations
The Gibbs free energy can then be calculat-ed using the following relation:
The thermodynamic parameters were deter-mined by considering desorption of β-carotene from samples 1, 2, and 3 under microwave irradia-tion at 303, 308, and 313 K; the results are present-ed in Table 4.
The obtained values of ΔG were positive, which suggests that β-carotene desorption is a non-spontaneous process. The low ΔG values obtained indicate that the mechanism of desorption may in-volve both a chemical and a physical process.
T a b l e 4
Thermodynamic parameters for desorption of β-carotene from bentonite adsorbents under microwave irradiation
ΔG (kJ mol–1) 303 K 308 K 313 K
83.9 245.6 53.04 19.61 9.77 8.32 6.71
In this study, β-carotene was desorbed from AABent saturated with different loading concen-trations under microwave irradiation at four
correspond-ed well with the prcorrespond-edictions of a first-order, two-component, three-parameter model.
The activation energies of β-carotene de-sorption for the rapid and slow dede-sorption process-es were 19.61 and 53.04 kJ mol–1, respectively. The activation energies depended on the adsorbent properties and the experimental conditions (mi-crowave irradiation).
The partition of β-carotene molecules be-tween the liquid phase and the adsorbent was fitted to the Langmuir and Freundlich models. Thermo-dynamic studies revealed that desorption of β -carotene from the bentonite adsorbents was non-spontaneous and endothermic in nature.
Acknowledgements. This work was supported by the
Ministry of Education and Science of the Republic of Serbia (Project number 172015).
 Y. Yuan, Y. Gao, L. Mao, J. Zhao, Optimization of con-ditions for the preparation of β-carotene nanoemulsions using response surface methodology, Food Chem.,107, 1300 (2008).
 A. Sanches-Silva, T. G. Albuquerque, P. Finglas, T. Ribeiro, A. Valente, E. Vasilopoulos, A. Trichopoulou, I. Alexieva, N. Boyko, C. E. Costra, O. Hayran, M. Jor-jadze, L. Kaprelyants, D. Karpenko, L. F. D'Antuoonom, H. S. Costaa, Carotenoids, vitamins (A, B2, C, and E),
and total folate of traditional foods from Black Sea Area countries, J. Sci. Food Agric.,93, 3545–3557 (2013).  S. C. Kheok, E. E. Lim, Mechanism of palm oil bleaching
by montmorillonite clay activated at various acid concen-trations, J. Am. Oil Chem. Soc.,59, 129–131 (1982).  E. Srasra, F. Bergaya, H. van Damme, N. K. Arguib,
Sur-face properties of an activated bentonite – decolorization of rapeseed oil, Appl. Clay Sci.,4, 411–421 (1989).  P. Falaras, I. Kovanis, F. Lezou, G. Seiragakis,
Cotton-seed oil bleaching by acid-activated montmorillonite,
Clay Miner.,34, 221–232 (1999).
 G. E. Christidis, S. Kosiari, Decolorization of vegetable oils: A study of the mechanism of adsorption of β -carotene by an acid-activated bentonite from Cyprus,
Clays Clay Miner., 51(3), 327–333 (2003).
 M. H. Ma, Ch. I. Lin, Adsorption kinetics of β-carotene from soybean oil using regenerated clay, Sep. Purif. Technol., 39, 201–209 (2004).
 E. Sabah, M. Çinar, M. S. Çelik, Decolorization of vege-table oils: Adsorption mechanism of β-carotene on acid-activated sepiolite, Food Chem., 100, 1661–1668 (2007).  M. Muhammad, T. S. Y. Choong, T. G. Chuah, R.
Yunus, Desorption of β-carotene from mesoporous car-bon-coated monolith: Isotherm, kinetics and regenera-tion studies, Chem. Eng. J., 173, 474–479 (2011).  M. Huang, Y. Xu, Q. Lv, Q. Ren, Separation and
purifi-cation of β-carotene from chlorophyll factory residues.,
Chem. Eng. Technol.,31(6), 922–927 (2008).
 Z. Wu, Ch. Li, Kinetics and thermodynamics of β -carotene and chlorophyll adsorption onto acid-activated
bentonite from Xinjiang in xylene solution, J Hazard. Mater., 171, 582–587 (2009).
 M. Muhammad, T. S. Y. Choong, T. G. Chuah, R. Yunus, Y. H. T. Yap, Adsorption of β-carotene onto mesoporous carbon coated monolith in isopropyl alcohol and n-hexane solution: Equilibrium and thermodynamic study, Chem. Eng. J.,164, 178–182 (2010).
 S. Petrović, Lj. Rožić, Z. Vuković, T. Novaković, D. Stanisavljev, Response surface optimization for activa-tion of bentonite with microwave irradiaactiva-tion, Clays Clay Miner.,60(1), 32–39 (2012).
 J. A. Menendez, A. Arenillas, B. Fidalgo, Y. Fernandez, L. Zubizrreta, E. G. Calvo, J. M. Bermudez, Microwave involving carbon materials, Fuel Process Technol., 91, 1–8 (2010).
 J. Li, Y. G. Zu, Y. J. Fu, Y. C. Yang, S. M. Li, Z. N. Li, M. Wink, Optimization of microwave-assisted extrac-tion of triterpene saponins from defated residue of yel-low horn (Xanthoceras sorbifolia Bunge) kernel and evaluation of its antioxidant activity, Innov. Food Sci. Emerg.,11, 637–643 (2010).
 G. Zhang, M. Hu, L. He, P. Fu, L. Wang, J. Zhou, Opti-mization of microwave-assisted enzymatic extraction of polyphenols from waste peanut shells and evaluation of its antioxidant and antibacterial activities in vitro, Food Bioprod. Process.,91, 158–168 (2013).
 B. Legras, I. Polert, M. Thomas, L. Estel, About using microwave irradiation in competitive adsorption pro-cesses, Appl. Therm. Engi., 57, 164–171 (2013).  R. Cherbanski, E. Molga, Intensification of desorption
processes by use of microwaves: An overview of possi-ble applications and industrial perspectives, Chem. Eng. Process., 48(1), 48–58 (2009).
 S. Ramesh, B. S. Jai Prakash, Y. S. Bhat, Enhancing Brønsted acid site activity of ion-exchanged montmoril-lonite by microwave irradiation for ester synthesis, Appl. Clay Sci.,48, 159–163 (2010).
 Lj. Rožić, T. Novaković, S. Petrović, Modelling and optimization process parameters of acid activation of bentonite by response surface methodology, Appl. Clay Sci., 48, 154–158 (2010).
 E. P. Barrett, L. G. Joyner, P. H. Halenda, The determi-nation of pore volume and area distributions in porous substances. I. Computations from nitrogen isotherms, J Am. Chem. Soc.,73, 373–380 (1951).
 F. Rouquerol, J. Rouquerol, K. Sing, Adsorption by pow-ers and porous solids. In: Principles, Methodology and Applications, Academic Press, London, 1999, pp. 18–21.  M. D. Johnson, W. J. Weber, Rapid prediction of
long-term rates of contaminant desorption from soils and sed-iments, Environ. Sci. Technol.,35, 427–433 (2001).  R. A. K. Rao, M. A. Khan, B. H. Hameed,
Sorp-tion/desorption studies on some natural minerals for the removal of toxic organic pollutants from aqueous solu-tion, Chem. Eng. J.,152, 421–427 (2009).
 T. W. Weber, R. K. Chakkravorti, Pore and solid diffu-sion models for fixed bed adsorbers, AIChEJ, 20, 218– 228 (1974).